# this file is part of refractiveindex.info database
# refractiveindex.info database is in the public domain
# copyright and related rights waived via CC0 1.0

REFERENCES: "<a href=\"http://refractiveindex.info/download/data/2017/ohara_2017-11-30.agf\">OHARA Zemax catalog 2017-11-30</a> (obtained from <a href=\"http://www.ohara-inc.co.jp/en/product/optical/list/\">http://www.ohara-inc.co.jp</a>)<br>See also <a href=\"http://refractiveindex.info/download/data/2017/ohara_2017-11-30.pdf\">OHARA glass data sheets</a>"
COMMENTS: ""
DATA:
  - type: formula 3 
    range: 0.3 2.4
    coefficients: 2.234734 -0.0097856687 2 0.0098367633 -2 0.00021398416 -4 -1.4554893e-05 -6 8.7393721e-07 -8
  - type: tabulated k
    data: |
        0.300 1.7030E-06
        0.310 7.7636E-07
        0.320 3.8407E-07
        0.330 1.9906E-07
        0.340 1.0763E-07
        0.350 6.1959E-08
        0.360 3.7486E-08
        0.370 2.9592E-08
        0.380 3.6507E-08
        0.390 1.5557E-08
        0.400 1.2758E-08
        0.420 1.6753E-08
        0.440 1.4034E-08
        0.460 1.0998E-08
        0.480 7.6471E-09
        0.500 7.9657E-09
        0.550 8.7623E-09
        0.600 9.5589E-09
        0.650 1.0355E-08
        0.700 5.5732E-09
SPECS:
    n_is_absolute: false
    λ_is_vacuum: false
    temperature: 25.0 °C
    coefficients_of_thermal_dispersion: 3.189e-06 0.0 0.0 0.0 0.0 0.0
    n_d: 1.503779
    V_d: 66.814545
    glass_code: 504668
    glass_status: preferred
    density: 2.46 g/cm<sup>3</sup>
    coefficient_of_thermal_expansion_1: 6.2e-06 K<sup>-1</sup>
    coefficient_of_thermal_expansion_2: 7e-06 K<sup>-1</sup>
    ΔP_gF: -0.003
    acid_resistance: 1.0
    phosphate_resistance: 1.0
